Metal cation- and anion-induced assembly: structures and luminescent properties
Jin, Feng; Wang, Hui-Zhen; Zhang, Ying; Wang, Yang; Zhang, Jun; Kong, Lin; Hao, Fu-Ying; Yang, Jia-Xiang; Wu, Jie-Ying; Tian, Yu-Peng; Zhou, Hong-Ping; CrystEngComm 15 (2013) 3687–; doi:10.1039/c3ce26685k

data_7210687
_publ_section_title
;
 Metal cation- and anion-induced assembly: structures and luminescent
 properties
;
_journal_issue                   18
_journal_name_full               CrystEngComm
_journal_page_first              3687
_journal_paper_doi               10.1039/c3ce26685k
_journal_volume                  15
_journal_year                    2013
_chemical_formula_sum            'C27 H18 Hg N6 S2'
_chemical_formula_weight         691.18
_chemical_name_systematic
;
?
;
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.000(5)
_cell_angle_beta                 95.017(5)
_cell_angle_gamma                90.000(5)
_cell_formula_units_Z            4
_cell_length_a                   13.460(5)
_cell_length_b                   25.921(5)
_cell_length_c                   7.340(5)
_cell_measurement_temperature    298(2)
_cell_volume                     2551(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0360
_diffrn_reflns_av_sigmaI/netI    0.0341
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -30
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            17956
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.52
_exptl_absorpt_coefficient_mu    6.225
_exptl_absorpt_correction_T_max  0.3690
_exptl_absorpt_correction_T_min  0.2567
_exptl_crystal_density_diffrn    1.800
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1336
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.20
_refine_diff_density_max         0.867
_refine_diff_density_min         -0.569
_refine_diff_density_rms         0.088
_refine_ls_extinction_coef       0.00040(12)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.032
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     326
_refine_ls_number_reflns         4497
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.032
_refine_ls_R_factor_all          0.0334
_refine_ls_R_factor_gt           0.0264
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0346P)^2^+0.7745P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0650
_refine_ls_wR_factor_ref         0.0681
_reflns_number_gt                3873
_reflns_number_total             4497
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3ce26685k.txt
_cod_data_source_block           jf
_cod_database_code               7210687